Interactions between Graphene and Ionic Liquid Electrolyte ... Jing...Graphene Supercapacitor Ionic...
Embed Size (px)
Transcript of Interactions between Graphene and Ionic Liquid Electrolyte ... Jing...Graphene Supercapacitor Ionic...
Electrochimica Acta 197 (2016) 84–91
Interactions between Graphene and Ionic Liquid Electrolyte inSupercapacitors
Jing Lia,b, Jie Tanga,b,*, Jinshi Yuana, Kun Zhanga, Qingguo Shaoa, Yige Suna,b,Lu-Chang Qinc,d,*aNational Institute for Materials Science, 1-2-1 Sengen, Tsukuba, Ibaraki 305-0047, JapanbDoctoral Program in Materials Science and Engineering, University of Tsukuba, 1-1-1 Tennodai, Tsukuba, Ibaraki 305-0006, JapancNingbo Institute of Materials Technology and Engineering, Chinese Academy of Sciences, Ningbo 315201, ChinadDepartment of Physics and Astronomy, University of North Carolina at Chapel Hill, Chapel Hill, NC 27599-3255, USA
A R T I C L E I N F O
Article history:Received 14 December 2015Received in revised form 27 February 2016Accepted 6 March 2016Available online 8 March 2016
A B S T R A C T
The graphene material prepared by the chemical reduction method usually has oxygenic functionalgroups in it and such functional groups often result in interactions between the graphene electrode andthe electrolyte in supercapacitors. We have examined the existential form of interactions betweengraphene as the electrode and three kinds of ionic liquid, 1-ethyl-3-methylimidazolium bis(trifluoromethylsulfonyl) imide (EMI-TFSI), 1-ethyl-3-methylimidazolium tetrafluoroborate (EMI-BF4),and 1-methyl-1-propylpiperidinium bis (trifluoromethyl sulfonyl) imide (MPPp-TFSI), as the electrolyteof a supercapacitor. Mass spectroscopy (MS) and Fourier transform infrared spectroscopy (FT-IR) analysesconfirmed that the residual hydroxyl groups in graphene were transferred to EMI+ and TFSI� lost oxygenatoms to graphene, while little reaction took place in BF4� or MPPp+, during the process of charging. Thechemical reactions are suggested to contribute to the device capacitance while it is also one of the reasonsfor the decreased electrochemical stability window. In this study the highest energy density achievedusing the graphene electrode is 169 Wh kg�1 in MPPp-TFSI electrolyte charged to 4.4 V.
ã 2016 Elsevier Ltd. All rights reserved.
Contents lists available at ScienceDirect
journal homepa ge: www.elsev ier .com/locate /e lectacta
To meet the growing energy demand, many devices have beendeveloped for energy storage applications. To evaluate theperformance of an energy storage device, two quantities arecommonly used: the energy density and power density. Higherenergy density will lead to a longer service time and higher powerdensity means a shorter charging/discharging time. Comparedwith other energy storage devices, the merits of electric double-layer capacitors, which are also often called supercapacitors, aretheir high power density and long lifetime . To improve itsenergy density while keeping its high power density, variousstructures of carbon have been the material of choice for theelectrode [2–4]. In recent years, graphene has attracted a lot ofattention for the application as supercapacitor electrode materialdue to its excellent conductivity and large specific surface areaowing to its unique two-dimensional structure [5–9].
http://dx.doi.org/10.1016/j.electacta.2016.03.0360013-4686/ã 2016 Elsevier Ltd. All rights reserved.
However, there are still problems that have limited the furtherimprovement of energy density in supercapacitors with grapheneelectrodes. One is the re-stacking of graphene sheets due to the vander Waals attractions after reduction, which will decrease thespecific surface area . To solve this problem, single-wall carbonnanotubes (SWNTs) and graphene (SWNT/graphene) compositeshave been developed which exhibited great advantages as theactive material for supercapacitor electrodes [7,11].
Besides the electrode materials, the electrolyte will also have asignificant impact on the performance of supercapacitors. Variousionic liquids have been investigated as the electrolyte to takeadvantage of their wider electrochemical stability window[12–14]. The interactions between the carbon electrode and theionic liquid electrolyte also affect the electrochemical performanceof the supercapacitors. In particular, the oxygenic functionalgroups on the carbon electrode can involve substantial interfacialinteractions with the ionic liquid electrolyte as having beendemonstrated both experimentally and theoretically [14–19]. Inthis study, using mass spectroscopy (MS), Fourier transforminfrared spectroscopy (FT-IR), and electrochemical characteriza-tion techniques, we have examined three different ionic liquids toinvestigate their respective electrochemical reactions with the
J. Li et al. / Electrochimica Acta 197 (2016) 84–91 85
SWNT/graphene electrode when the ionic liquid was used as theelectrolyte in a symmetric supercapacitor: 1-ethyl-3-methylimi-dazolium bis (trifluoromethylsulfonyl) imide (EMI-TFSI), 1-ethyl-3-methylimidazolium tetrafluoroborate (EMI-BF4), and 1-methyl-1-propylpiperidinium bis (trifluoromethylsulfonyl) imide (MPPp-TFSI). The selection of these ionic liquids is largely due to theirwider electrochemical stability window and good electric conduc-tivity in comparison with other ionic liquids . Basing on theresults obtained in this study, a highest energy density of
Fig.1. Electrochemical stability window measured by three-electrode system with workiEMI-BF4, and (c) MPPp-TFSI. The inset in each figure shows the chemical structure of respthe reader is referred to the web version of this article.)
169 Wh kg�1 was achieved for the graphene electrode in asymmetric supercapacitor charged to 4.4 V using MPPp-TFSI asthe electrolyte.
Graphene oxide (GO) was prepared from graphite using theHummers method . Single-wall carbon nanotubes were firstdispersed by sonication in distilled water using sodium
ng electrode Pt (colored black) and SWNT/graphene (colored red) in (a) EMI-TFSI, (b)ective ionic liquid. (For interpretation of the references to color in this figure legend,
86 J. Li et al. / Electrochimica Acta 197 (2016) 84–91
dodecylbenzenesulfonate (SDBS) as surfactant. SWNT/GO com-posite was then prepared by mixing the dispersions of SWNT andGO powders before it was reduced by hydrazine at 98 �C for24 hours. The reduced material was rinsed with water and filteredfor several times until it became neutral after removing SDBS. TheSWNT/graphene composite was eventually obtained as blackpowders. The coin cell supercapacitor was assembled in thestructure as illustrated in Fig. S1 (Supplementary Information).
The ionic liquids with purity 99.9% were purchased commer-cially (EMI-TFSI from Solvionic, EMI-BF4 and MPPp-TFSI from Toyo-Gosei). The chemical structure of the ionic liquids was character-ized by mass spectroscopy (MS) using AMR Zaplous LC/MS Systemand Fourier transform infrared spectroscopy (FT-IR) using JASCOFT/IR-6100.
Fig. S1 (Supplementary Information) shows schematically thepreparation of electrolyte samples for MS and FT-IR characteriza-tion. After completing the charging-discharging process, theelectrolyte sample was extracted from the disassembled coin cellsupercapacitor using a syringe. For FT-IR characterization, theextracted electrolyte was used directly. For MS characterization,the extracted electrolyte was diluted with acetone to a concentra-tion of 0.2 mol L�1.
The electrode samples were taken directly from the dissembledthe coin cell supercapacitor and they were rinsed in acetone anddried in vacuum. The functional groups on the electrode surfacewere characterized using x-ray photoelectron spectroscopy (XPS;ULVAC-PHI Quantera SXM) with a twin anode Al Ka x-ray sourceand hemispherical energy analyzer. The energies were calibratedagainst the aliphatic carbon C1s peak at 284.5 eV.
Electrochemical characterization was carried out using a multi-channel VMP-300 electrochemical workstation.
In order to find out the threshold voltage beyond whichelectrochemical reactions take place between the ionic liquidelectrolyte and the SWNT/graphene electrode during charging, theelectrochemical stability window was measured using a three-electrode system with Pt as the counter electrode, silver-silver ion(Ag/Ag+) as the reference electrode, and Pt or SWNT/graphenecomposite as the working electrode, respectively. To avoid theinterference of water and oxygen in the air, the measurement wascarried out in a glove box.
3. Results and Discussion
3.1. Reactions in Electrolyte
Fig. 1 shows the plot of current (mA) vs. voltage (V) acquiredexperimentally for the three different ionic liquid electrolytes andthe results are also summarized in Table 1. The electrochemicalstability window herein refers to the range of applied potentials inwhich no electrochemical reactions would take place. When theworking electrode is Pt, the inflection points on the I–V curves(colored black) are due to the decomposition of the ionic liquidelectrolyte and therefore the corresponding voltage is the
Table 1Electrochemical stability window of ionic liquid electrolyte for Pt and SWNT/graphene working electrode.
Electrolytes Working Electrode Electrochemical Window
EMI-TFSI Pt �2.5 V � 2.1 V (D=4.6 V)EMI-TFSI SWNT/Graphene �2.4 V � 1.3 V (D=3.7 V)EMI-BF4 Pt �2.8 V � 1.8 V (D=4.6 V)EMI-BF4 SWNT/Graphene �2.3 V � 1.4 V (D=3.7 V)MPPp-TFSI Pt �3.4 V � 2.4 V (D=5.8 V)MPPp-TFSI SWNT/Graphene �2.4 V � 1.6 V (D=4.0 V)
decomposition voltage for each of the three ion liquids: (a) EMI-TFSI (4.6 V), (b) EMI-BF4 (4.6 V), and (c) MPPp-TFSI (5.8 V) .However, in the same ionic liquid, the inflection point (colored red)started to appear before the electrode reached the decompositionvoltage when the SWNT/graphene composite was used as theworking electrode as shown in the I–V curves (colored red) in Fig.1.The inflection points on the red curves are therefore attributed tothe electrochemical reactions between the ionic liquid electrolyteand the SWNT/graphene electrode .
As indicated in Fig. 1 and Table 1, electrochemical reactionsbetween the SWNT/graphene electrode and the EMI-TFSI or EMI-BF4 ionic liquid would occur when the voltage between the twoelectrodes was in the range of 3.7 and 4.6 V. Electrochemicalreactions would occur between the SWNT/graphene electrode andthe MPPp-TFSI electrolyte when the voltage between the twoelectrodes was in the range of 4.0 and 5.8 V using ionic liquidelectrolyte MPPp-TFSI.
To study the electrochemical reactions occurred to the EMI-TFSIionic liquid electrolyte in the charged supercapacitor, we examinedthe electrolyte that was extracted from the coin cell supercapacitorafter it was charged to 4.0 V. Fig. 2 shows the mass spectrum of theextracted electrolyte together with the mass spectrum of pristineionic liquid EMI-TFSI. As expected, there are only two peaks in themass spectrum (Fig. 2(a)) of pristine EMI-TFSI with mass-to-chargeratio (m/z) of 111 and 280, corresponding to the EMI+ and TFSI�
ions, respectively . However, there appeared two additionalpeaks in the spectrum of used electrolyte (Fig. 2(b)), indicatingnew products from the electrochemical reactions in used EMI-TFSI.According to the changed mass of the ion from 111 to 129, the newpeak at 129 is attributed to an addition to EMI+ of a hydroxyl group(-OH + H) broken away from the graphene electrode  and thenew peak at 264 is attributed to the TFSI� ion losing an oxygenatom, as illustrated in Fig. 3.
To elucidate the chemical nature of the associated changes inthe mass of the ions, we employed Fourier transform infraredspectroscopy (FT-IR) to characterize the functional groups. Thealkyl C-H stretching peak (2980 cm�1) was normalized as thereference for comparison . In the spectrum of EMI-TFSI (Fig. 4),it can be seen that the peak height corresponding to the doublebond between sulfur and oxygen (S¼O) decreased after charging.Since TFSI� is the only source of S¼O bond, it indicates that TFSI�lost oxygen atoms due to breakage of the S¼O bond, which is inagreement with the MS analysis. Moreover, the spectrum alsoshowed that a new peak corresponding to the single bond betweenO and H (O-H) appeared after charging, indicating that certainhydroxyl groups were added to EMI-TFSI. It also agrees well withthe MS analysis described above.
Characterization and analysis were also carried out on thepristine EMI-BF4 and the used EMI-BF4 electrolyte extracted from acoin cell supercapacitor after charging to 4.2 V. The MS data of EMI-BF4 before and after charging are shown in Fig. 5. The cation, EMI+,tends to form a dimer in EMI-BF4, which results in the peak at308 in the spectrum of pristine EMI-BF4 [16,24]. Similarly, since thecation in EMI-BF4 is the same as that in EMI-TFSI, the peak at129 also showed up after charging, indicating that a hydroxylgroup had been acquired by EMI+. However, no additional peakrelated to reaction with BF4� was observed. It is thereforesuggested that there were no electrochemical reaction betweenBF4� and the SWNT/graphene electrode under charging. It is asignificant difference from TFSI�.
More details are reflected in the FT-IR spectrum of EMI-BF4(Fig. 6). Compared with EMI-TFSI, when the anion of the ionicliquid was changed to BF4�, the peak corresponding to the singlebond between O and H (O-H) still showed up in the extractedelectrolyte after charging. It supports the assumption that thehydroxyl groups are connected to EMI+, rather than BF4� or TFSI.
Fig. 2. MS data of EMI-TFSI (a) before and (b) after charging. The new peaks at 129 and 264 in the spectrum (b) after charging indicate additional products from theelectrochemical reactions between EMI-TFSI and the SWNT/graphene electrode.
Fig. 3. Schematic of reactions between EMI-TFSI and graphene. Hydroxyl groups from graphene are added to EMI+ while TFSI� loses oxygen atoms to graphene.
J. Li et al. / Electrochimica Acta 197 (2016) 84–91 87
When using MPPp-TFSI as the electrolyte and comparing withEMI-TFSI, the cation was changed to MPPp+ and the peak at 280 inthe MS spectrum (Fig. 7) did not disappear after charging. Ittherefore indicates that the additional product corresponding tothe peak is from electrochemical reactions with TFSI�, rather thanEMI+ or MPPp+. In addition, there was no additional peak arisenfrom electrochemical reactions related to MPPp+.
Fig. 8 shows the FT-IR data of MPPp-TFSI before and aftercharging, which agrees with the MS analysis. There was no peakarisen in the range of 3000 and 4000 cm�1 after charging,indicating that the hydroxyl groups on the electrode had littlereaction with MPPp+ or TFSI�.
The hydroxyl radicals (�OH) and hydrions are assumed to form atthe edgesof graphene and carbon nanotubes athighvoltage and then
Fig. 4. FT-IR data of EMI-TFSI before and after charging. The peak in the range of 3500 andecrease of the S¼O peak after charging indicates that TFSI� loses oxygen atoms as S¼
�OH would attack the electropositive imidazole ring to have itattached to EMI+ [25,27,28]. For the loss of sulfonyl oxygen in TFSI�,the S¼O bond mightbeprotonatedto S-OH first and then �OHwouldattack the attached heteroatoms in graphene and carbon nanotubeswhile breaking-up the S-O bond at the same time [28–32].
3.2. Reactions on Electrode
Besides the electrolyte, electrochemical reactions also occurredon the SWNT/graphene electrode, which would in turn affect theperformance of the graphene supercapacitor. FT-IR and XPS wereapplied to analyze the electrochemical reactions occurred on theSWNT/graphene electrode, which was taken out from the coin cellsupercapacitor after charging. Results of analysis were compared
d 3700 cm�1 indicates existence of hydroxyl groups in EMI-TFSI after charging. TheO bond breakage occurrs.
Fig. 5. MS data of EMI-BF4 (a) before and (b) after charging. The peak at 129 is due to reaction with EMI+ after acquiring a hydroxyl group.
88 J. Li et al. / Electrochimica Acta 197 (2016) 84–91
before and after charging of the SWNT/graphene electrode in orderto find out the differences of the functional groups on the SWNT/graphene electrode using different ionic liquid electrolyte.
Fig. 9 shows the FT-IR data taken from the graphene electrodebefore and after charging from 0 to 4.0 V in EMI-TFSI electrolyte. Inthe spectrum the intensity of the peak corresponding to the bondbetween the carbon atoms (C¼C) in the hexatomic ring isnormalized as the reference for comparison. It can be seen thatthe peaks corresponding to the single bond between carbon andoxygen (C-O) and the single bond between oxygen and hydrogen(O-H) on the electrode decreased more than 50%, while the peakcorresponding to the double bond between carbon and oxygen(C¼O) increased after charging in the EMI-TFSI electrolyte.Combining with the FT-IR analysis of EMI-TFSI, we suggest thatthe reduced peaks are due to the breakage of bonds between thehydroxyl groups and carbon atoms on the SWNT/grapheneelectrode and that the detached hydroxyl groups were added toEMI-TFSI. At the same time, the lost oxygen atoms from TFSI�
became associated with the carbon atoms in SWNT/graphene bydouble bond, which resulted in an increase of the correspondingpeak in the FT-IR spectrum.
As for the ionic electrolyte EMI-BF4, as shown in Fig.10, the peakcorresponding to the single bond between oxygen and hydrogen(O-H) decreased after charging, which is similar to the results inEMI-TFSI. It is attributed to a reaction in which the hydroxyl groupfrom graphene is captured by EMI+ under charging. At the sametime, the peak due to the double bond between carbon and oxygen
Fig. 6. FT-IR of EMI-BF4 before and after charging. More hydroxyl groups areobserved after charging.
(C¼O) in graphene stayed unchanged after charging, different fromthe graphene electrode charged in EMI-TFSI. Combining with theMS results, it showed that EMI-BF4 had little reaction with thefunctional groups on graphene.
Different from graphene electrode charged in EMI-TFSI andEMI-BF4, the FT-IR (Fig. 11) results showed that the peakcorresponding to the single bond between oxygen and hydrogen(O-H) remained the same after charging in the MPPp-TFSIelectrolyte. It therefore indicates that the reduction of hydroxylgroups on the SWNT/graphene electrode is due to reactions withEMI+ rather than MPPp+.
Fig. S2 (Supplementary Information) shows the C1s spectra ofthe parent SWNT/graphene electrode and the activated electrodeafter electrochemical loading. The decreased ratio of C-OH peak at285.6 eV in electrode charged in EMI-TFSI and EMI-BF4 supple-ments the FT-IR results . Besides, the O/C ratio increased from22.8% to 27.7% after charging in MPPp-TFSI. Combining with thecharacterization results of the electrolyte, the increased oxygen onthe SWNT/graphene electrode is attributed to the breakage of theS¼O bond in TFSI�.
Given the close similarity in bonding between the carbonatoms, it should be noted that the electrochemical reactionsdiscussed above could take place in both graphene and SWNTsinterchangeably.
3.3. Influence on Performance of Supercapacitor
In the cyclic voltammetry (CV) measurement, a chemicalreaction would result in a sudden change in the electric current,which is reflected as a redox peak on the CV curve. From the CVdiagram, we can therefore expect that, when the voltage appliedon the supercapacitor is larger than 3.7 V, redox peaks couldappear on the CV curves for EMI-TFSI and EMI-BF4 electrolyte dueto the occurrence of chemical reactions.
However, redox peaks also appeared on the CV curves withMPPp-TFSI electrolyte even when the applied voltage was smallerthan the threshold voltage required for chemical reactions withMPPp-TFSI (4.0 V). These redox peaks are attributed to the physicalinteractions between the electrolyte ions and the structural poresin the active material of the electrode [33–35]. Considering the factthat the size of MPPp+ is larger than EMI+, chemical reactions maybe not the only interaction between MPPp-TFSI and graphene .Physical interactions between pores and ions in MPPp-TFSIelectrolyte are also possible to take a dominant role in the twokinds of interactions, resulting in the peaks on the CV curves ofMPPp-TFSI subjected to a lower voltage. For example, penetrationof ions into the pores smaller than the ions is possible [36,37].
Fig. 7. MS data of MPPp-TFSI (a) before and (b) after charging. The peak at 264 is due to reaction with TFSI� after it loses an oxygen atom.
Fig. 8. FT-IR data of MPPp-TFSI before and after charging. No significant change dueto charging is observed.
Fig. 9. FT-IR data of SWNT/graphene electrode before and after charging in EMI-TFSI. The peak corresponding to the hydroxyl group has an obvious drop, indicatingthat some of the hydroxyl groups were removed from the graphene electrode aftercharging.
J. Li et al. / Electrochimica Acta 197 (2016) 84–91 89
Table 2 lists the specific capacitance and energy density of thegraphene supercapacitor calculated from the charge-dischargecurves (Fig. 12) at the current density of 0.2 A g�1. The super-capacitor with EMI-TFSI electrolyte has a larger specific capaci-tance under the same charged voltage. Considering that there are
Fig. 10. FT-IR data of SWNT/graphene electrode before and after charging in EMI-BF4 electrolyte.
more reactions between EMI-TFSI and graphene, it implies that thechemical species due to both the ionic liquid and the grapheneelectrode contributed to the larger capacitance. On the other hand,the largest energy density was achieved in the supercapacitorusing the MPPp-TFSI electrolyte when the applied voltage reached4.4 V. Even though the specific capacitance with MPPp-TFSIelectrolyte is smaller than that with EMI-TFSI and EMI-BF4electrolyte, the electrochemical stability window and thereforethe operating voltage is larger with the MPPp-TFSI electrolyte tolead to the highest energy density of 169 Wh kg�1.
Measurement of electrochemical stability windows revealedthat electrochemical reactions took place between the ionic liquidelectrolyte and the SWNT/graphene electrode when the appliedvoltage was in the range of 3.7 and 4.6 V for EMI-TFSI and EMI-BF4.For MPPp-TFSI electrolyte, electrochemical reactions occurred inthe range of 4.0 and 5.8 V. Using mass spectroscopy and Fouriertransform infrared spectroscopy, we determined that the hydroxylgroups from SWNT/graphene were transferred to EMI+ and TFSI�
would lose oxygen atoms to SWNT/graphene during charging,while little reaction occurred to BF4� and MPPp+.
The electrochemical reactions will affect the performance ofgraphene supercapacitors and they are one of the reasons for the
Fig. 11. FT-IR data of SWNT/graphene electrode before and after charging in MPPp-TFSI electrolyte.
Table 2Performance of graphene supercapacitors with different ionicliquid electrolyte.
3.7 EMI-TFSI 243 112EMI-BF4 174 81MPPp-TFSI
4.0 EMI-TFSI 332 156EMI-BF4 197 105MPPp-TFSI
4.2 EMI-BF4 260 145MPPp-TFSI
Fig. 12. CV of supercapacitor with (a) EMI-TFSI, (b), EMI-BF4, and (c) MPPp-TFSI electrolyte. The corresponding charge-discharge curves measured at current density of0.2 A g�1 are given in (d-f).
90 J. Li et al. / Electrochimica Acta 197 (2016) 84–91
J. Li et al. / Electrochimica Acta 197 (2016) 84–91 91
decreased electrochemical stability window. The largest specificcapacitance under the same voltage was achieved in EMI-TFSIelectrolyte while the highest energy density of 169 Wh kg�1 wasachieved in MPPp-TFSI electrolyte due to a higher operatingvoltage of 4.4 V.
This work was financially supported by the JST ALCA Program(No. 22310074), JSPS Grants-in-Aid for Scientific Research (No.22310074), the Nanotechnology Network Project of MEXT, Japan,and Provincial Natural Science Foundation (No. LY14E020010) ofZhejiang, China.
Appendix A. Supplementary data
Supplementary data associated with this article can befound, in the online version, at http://dx.doi.org/10.1016/j.electacta.2016.03.036.
 G.P. Wang, L. Zhang, J.J. Zhang, Chem. Soc. Rev. 41 (2012) 797–828. L.L. Zhang, X.S. Zhao, Chem. Soc. Rev. 38 (2009) 2520–2531. M. Liang, F.M. Jin, R. Liu, R.X. Su, W. Qi, Y.J. Yu, L.B. Wang, Z.M. He, J. Mater. Sci.
48 (2013) 5624–5632. H. Pan, J.Y. Li, Y.P. Feng, Nanoscale Res. Lett. 5 (2010) 654–668. L.M. Dai, D.W. Chang, J.-B. Baek, W. Lu, Small 8 (2012) 1130–1166. C.G. Liu, Z.N. Yu, D. Neff, A. Zhamu, B.Z. Jang, Nano Lett. 10 (2010) 4863–4868. Q. Cheng, J. Tang, J. Ma, H. Zhang, N. Shinya, L.-C. Qin, Phys. Chem. Chem. Phys.
13 (2011) 17615–17624. J.B. Hou, Y.Y. Shao, M.W. Ellis, R.B. Moored, B.L. Yi, Phys. Chem. Chem. Phys. 13
(2011) 15384–15402. D.R. Dreyer, S. Park, C.W. Bielawski, R.S. Ruoff, Chem. Soc. Rev. 39 (2010) 228–
240. J. Yan, T. Wei, B. Shao, F.Q. Ma, Z.J. Fan, M.L. Zhang, C. Zheng, Y.C. Shang, W.Z.
Qian, F. Wei, Carbon 48 (2010) 1731–1737. F.F. Zhang, J. Tang, N. Shinya, L.-C. Qin, Chem. Phys. Lett. 584 (2013) 124–129.
 M. Armand, F. Endres, D. R. MacFarlane, H. Ohno, and B. Scrosati, Nature Mater.8 (2009) 621–629. K. P. Gong, S. Chakrabarti, and L. M. Dai, Angew. Chem. Int.Ed. 47 (2008) 5446–5450.
 R. Kotz, M. Carlen, Electrochim. Acta 45 (2000) 2483–2498. M. Vijayakumar, B. Schwenzer, V. Shutthanandan, J.Z. Hu, J. Liu, I.A. Aksay,
Nano Energy 3 (2014) 152–158. S. Kerisit, B. Schwenzer, M. Vijayakumar, J. Phys. Chem. Lett. 5 (2014) 2330–
2334. T. Romann, O. Oll, P. Pikma, H. Tamme, E. Lust, Electrochim. Acta 125 (2014)
183–190. W. Ai, X.H. Cao, Z.P. Sun, J. Jiang, Z.Z. Du, L.H. Xie, Y.L. Wang, X.J. Wang, H. Zhang,
W. Huang, T. Yu, J. Mater. Chem. A 2 (2014) 12924–12930. Y.S. Ye, H. Wang, S.G. Bi, Y. Xue, Z.G. Xue, Y.G. Liao, X.P. Zhou, X.L. Xie, Y.W. Mai,
Carbon 86 (2015) 86–97. Q. Shao, J. Tang, Y. Lin, J. Li, F. Qin, K. Zhang, J. Yuan, L.-C. Qin, Electrochim. Acta
176 (2015) 1441–1446. S. Zhang, N. Sun, X. He, X. Lu, X. Zhang, J. Phys. Chem. Ref. Data 35 (2006) 1475–
1517. W.S. Hummers, R.E. Offeman, J. Am. Chem. Soc. 80 (1958) 1339. G.B. Appetecchi, M. Montaninoa, D. Zaneb, M. Carewska, F. Alessandrini, S.
Passerini, Electrochim. Acta 54 (2009) 1325–1332. X.Z. Yuan, V. Alzate, Z. Xie, D.G. Ivey, E. Dy, W. Qua, J. Electrochem. Soc. 161
(2014) 458–466. C.Y. Kong, W.Z. Qian, C. Zheng, Y.T. Yu, C.J. Cui, F. Wei, Chem. Commun. 49
(2013) 10727–10729. J. Llano, L.A. Eriksson, J. Phys. Chem. B 103 (1999) 5598–5607. X. Chen, J. Zhao, J. Zhang, L. Qiu, D. Xu, H. Zhang, X. Han, B. Sun, G. Fu, Y. Zhang,
F. Yan, J. Mater. Chem. 22 (2012) 18018–18024. T. Kuila, A.K. Mishra, P. Khanra, N.H. Kim, J.H. Lee, Nanoscale 5 (2013) 52–71. L. Chen, Y. Tang, K. Wang, C. Liu, S. Luo, Electrochem. Commun. 13 (2011) 133–
137. R.L. Carlson, R.S. Drago, J. Am. Chem. Soc. 84 (1962) 2320–2323. W. Ying, D.D. DesMarteau, Y. Gotoh, Tetrahedron 52 (1996) 15–22. P. Kielbasinski, J. Drabowicz, M. Mikolajczyk, J. Org. Chem. 47 (1982) 4806–
4808. J.-C. Lassegues, J. Grondin, C. Aupetit, P. Johansson, J. Phys. Chem. A 113 (2009)
305–314. H.-C. Huang, C.-W. Huang, C.-T. Hsieh, H. Teng, J. Mater. Chem. A 2 (2014)
14963–14972. J. Chmiola, C. Largeot, P.-L. Taberna, P. Simon, Y. Gogotsi, Angew. Chem. Int. Ed.
47 (2008) 3392–3395. A. Bhattacharjee, P.J. Carvalho, J.A.P. Coutinho, Fluid Phase Equilibria 375
(2014) 80–88. H. Zhang, G. Cao, Y. Yang, Z. Gu, J. Electrochem. Soc. 155 (2008) 19–22. C.-M. Yang, H.J. Jung, Y.J. Kim, J. Colloid Interface Sci. 446 (2015) 208-2.
Interactions between Graphene and Ionic Liquid Electrolyte in Supercapacitors1 Introduction2 Experimental3 Results and Discussion3.1 Reactions in Electrolyte3.2 Reactions on Electrode3.3 Influence on Performance of Supercapacitor
4 ConclusionsAcknowledgementsAppendix A Supplementary dataReferences